#------------------------------------------------------------------------------
#$Date: 2016-03-23 00:24:52 +0200 (Wed, 23 Mar 2016) $
#$Revision: 179109 $
#$URL: svn://www.crystallography.net/cod/cif/4/30/71/4307161.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_4307161
loop_
_publ_author_name
'William R. Gemmill'
'Mark D. Smith'
'Hans-Conrad zur Loye'
_publ_section_title
;
Ln14Na3Ru6O36 (Ln = Pr, Nd): Two New Complex Lanthanide-Containing Oxides
of Ruthenium
;
_journal_name_full               'Inorganic Chemistry'
_journal_page_first              2132
_journal_page_last               2138
_journal_paper_doi               10.1021/ic0617083
_journal_volume                  46
_journal_year                    2007
_chemical_formula_moiety         'Na3 O36 Pr14 Ru6'
_chemical_formula_sum            'Na3 O36 Pr14 Ru6'
_chemical_formula_weight         3224.13
_chemical_name_systematic
; 
 ? 
;
_space_group_IT_number           167
_symmetry_cell_setting           trigonal
_symmetry_space_group_name_Hall  '-R 3 2"c'
_symmetry_space_group_name_H-M   'R -3 c :H'
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                120.00
_cell_formula_units_Z            6
_cell_length_a                   9.7380(2)
_cell_length_b                   9.7380(2)
_cell_length_c                   55.5716(15)
_cell_measurement_reflns_used    4433
_cell_measurement_temperature    294(2)
_cell_measurement_theta_max      32.539
_cell_measurement_theta_min      2.828
_cell_volume                     4563.76(18)
_computing_cell_refinement       'SAINT+ NT V6.22 (Bruker, 2001)'
_computing_data_collection       'SMART NT V5.628 (Bruker, 2001)'
_computing_data_reduction        'SAINT+ NT V6.22'
_computing_molecular_graphics    'SHELXTL V6.1 (Sheldrick, 2000)'
_computing_publication_material  'SHELXTL V6.1'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      294(2)
_diffrn_measured_fraction_theta_full 0.999
_diffrn_measured_fraction_theta_max 0.999
_diffrn_measurement_device_type  'Bruker SMART APEX CCD diffractometer'
_diffrn_measurement_method       'omega scans'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0751
_diffrn_reflns_av_sigmaI/netI    0.0357
_diffrn_reflns_limit_h_max       14
_diffrn_reflns_limit_h_min       -14
_diffrn_reflns_limit_k_max       14
_diffrn_reflns_limit_k_min       -14
_diffrn_reflns_limit_l_max       83
_diffrn_reflns_limit_l_min       -84
_diffrn_reflns_number            19736
_diffrn_reflns_theta_full        32.57
_diffrn_reflns_theta_max         32.57
_diffrn_reflns_theta_min         2.20
_diffrn_standards_decay_%        0
_exptl_absorpt_coefficient_mu    24.974
_exptl_absorpt_correction_T_max  1.0000
_exptl_absorpt_correction_T_min  0.4708
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   'SADABS (Bruker, 2001)'
_exptl_crystal_colour            black
_exptl_crystal_density_diffrn    7.039
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       irregular
_exptl_crystal_F_000             8466
_exptl_crystal_size_max          0.05
_exptl_crystal_size_mid          0.04
_exptl_crystal_size_min          0.03
_refine_diff_density_max         1.663
_refine_diff_density_min         -4.122
_refine_diff_density_rms         0.530
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.087
_refine_ls_matrix_type           full
_refine_ls_number_parameters     91
_refine_ls_number_reflns         1855
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.087
_refine_ls_R_factor_all          0.0417
_refine_ls_R_factor_gt           0.0368
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.0145P)²+576.4727P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0727
_refine_ls_wR_factor_ref         0.0744
_reflns_number_gt                1724
_reflns_number_total             1855
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            ic0617083rom20060908_043430.cif
_cod_data_source_block           wg2059as
_cod_depositor_comments
;
The following automatic conversions were performed:
'_symmetry_cell_setting' value 'Trigonal' changed to 'trigonal' according
to '/home/saulius/struct/CIF-dictionaries/cif_core.dic' dictionary named
'cif_core.dic' version 2.4.1 from 2010-06-29.

Automatic conversion script
Id: cif_fix_enum 1527 2010-12-29 10:47:43Z saulius 
;
_cod_original_sg_symbol_H-M      'R -3 c'
_cod_database_code               4307161
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-y, x-y, z'
'-x+y, -x, z'
'y, x, -z+1/2'
'x-y, -y, -z+1/2'
'-x, -x+y, -z+1/2'
'x+2/3, y+1/3, z+1/3'
'-y+2/3, x-y+1/3, z+1/3'
'-x+y+2/3, -x+1/3, z+1/3'
'y+2/3, x+1/3, -z+5/6'
'x-y+2/3, -y+1/3, -z+5/6'
'-x+2/3, -x+y+1/3, -z+5/6'
'x+1/3, y+2/3, z+2/3'
'-y+1/3, x-y+2/3, z+2/3'
'-x+y+1/3, -x+2/3, z+2/3'
'y+1/3, x+2/3, -z+7/6'
'x-y+1/3, -y+2/3, -z+7/6'
'-x+1/3, -x+y+2/3, -z+7/6'
'-x, -y, -z'
'y, -x+y, -z'
'x-y, x, -z'
'-y, -x, z-1/2'
'-x+y, y, z-1/2'
'x, x-y, z-1/2'
'-x+2/3, -y+1/3, -z+1/3'
'y+2/3, -x+y+1/3, -z+1/3'
'x-y+2/3, x+1/3, -z+1/3'
'-y+2/3, -x+1/3, z-1/6'
'-x+y+2/3, y+1/3, z-1/6'
'x+2/3, x-y+1/3, z-1/6'
'-x+1/3, -y+2/3, -z+2/3'
'y+1/3, -x+y+2/3, -z+2/3'
'x-y+1/3, x+2/3, -z+2/3'
'-y+1/3, -x+2/3, z+1/6'
'-x+y+1/3, y+2/3, z+1/6'
'x+1/3, x-y+2/3, z+1/6'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
_atom_site_disorder_assembly
_atom_site_disorder_group
Pr1 Pr 0.00471(5) 0.28850(5) 0.216615(7) 0.00525(9) Uani 1 1 d . . .
Pr2 Pr 0.02893(5) 0.34290(5) 0.147833(8) 0.00642(10) Uani 1 1 d . . .
Pr3 Pr 0.0000 0.0000 0.107956(13) 0.00587(14) Uani 1 3 d S . .
Ru1 Ru -0.00050(8) 0.3333 0.0833 0.00193(14) Uani 1 2 d S . .
Ru2 Ru 0.0000 0.0000 0.0000 0.0032(2) Uani 1 6 d S . .
Ru3 Ru 0.0000 0.0000 0.162491(17) 0.00280(17) Uani 1 3 d S . .
Na1 Na 0.0000 0.0000 0.2500 0.0087(15) Uani 1 6 d S . .
Na2 Na 0.0000 0.0000 0.05338(11) 0.0125(11) Uani 1 3 d S . .
O1 O 0.1976(7) 0.1916(7) 0.22402(10) 0.0068(10) Uani 1 1 d . . .
O2 O 0.1954(7) 0.1296(7) 0.14128(10) 0.0094(10) Uani 1 1 d . . .
O3 O 0.0655(7) 0.1983(7) 0.17956(10) 0.0076(10) Uani 1 1 d . . .
O4 O 0.2338(7) 0.1349(7) 0.08171(10) 0.0074(10) Uani 1 1 d . . .
O5 O 0.1443(7) 0.3554(7) 0.05777(10) 0.0072(10) Uani 1 1 d . . .
O6 O 0.1660(7) 0.1703(7) 0.02056(11) 0.0097(11) Uani 1 1 d . . .
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Na Na 0.0362 0.0249 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Ru Ru -1.2594 0.8363 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Pr Pr -0.2180 2.8214 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
O2 Pr1 O3 80.4(2) 26_455 . ?
O2 Pr1 O4 147.74(19) 26_455 34 ?
O3 Pr1 O4 124.21(19) . 34 ?
O2 Pr1 O5 72.5(2) 26_455 34 ?
O3 Pr1 O5 130.10(19) . 34 ?
O4 Pr1 O5 75.44(18) 34 34 ?
O2 Pr1 O6 80.9(2) 26_455 34 ?
O3 Pr1 O6 65.1(2) . 34 ?
O4 Pr1 O6 91.0(2) 34 34 ?
O5 Pr1 O6 69.72(19) 34 34 ?
O2 Pr1 O1 81.24(19) 26_455 2 ?
O3 Pr1 O1 86.07(19) . 2 ?
O4 Pr1 O1 117.59(19) 34 2 ?
O5 Pr1 O1 128.29(19) 34 2 ?
O6 Pr1 O1 148.2(2) 34 2 ?
O2 Pr1 O1 145.92(19) 26_455 . ?
O3 Pr1 O1 68.94(19) . . ?
O4 Pr1 O1 66.00(18) 34 . ?
O5 Pr1 O1 139.63(19) 34 . ?
O6 Pr1 O1 98.66(19) 34 . ?
O1 Pr1 O1 82.1(3) 2 . ?
O2 Pr1 O4 83.26(18) 26_455 26_455 ?
O3 Pr1 O4 148.21(18) . 26_455 ?
O4 Pr1 O4 82.4(2) 34 26_455 ?
O5 Pr1 O4 68.73(18) 34 26_455 ?
O6 Pr1 O4 138.27(18) 34 26_455 ?
O1 Pr1 O4 64.52(17) 2 26_455 ?
O1 Pr1 O4 115.48(17) . 26_455 ?
O2 Pr1 Na1 126.53(14) 26_455 . ?
O3 Pr1 Na1 94.01(14) . . ?
O4 Pr1 Na1 76.46(13) 34 . ?
O5 Pr1 Na1 135.76(13) 34 . ?
O6 Pr1 Na1 143.86(14) 34 . ?
O1 Pr1 Na1 45.30(13) 2 . ?
O1 Pr1 Na1 45.24(13) . . ?
O4 Pr1 Na1 74.29(12) 26_455 . ?
O2 Pr1 Na2 114.77(15) 26_455 34 ?
O3 Pr1 Na2 99.69(16) . 34 ?
O4 Pr1 Na2 46.73(16) 34 34 ?
O5 Pr1 Na2 58.38(14) 34 34 ?
O6 Pr1 Na2 44.91(17) 34 34 ?
O1 Pr1 Na2 163.60(15) 2 34 ?
O1 Pr1 Na2 85.64(13) . 34 ?
O4 Pr1 Na2 111.92(15) 26_455 34 ?
Na1 Pr1 Na2 118.57(7) . 34 ?
O2 Pr1 Ru1 176.18(14) 26_455 27 ?
O3 Pr1 Ru1 96.93(14) . 27 ?
O4 Pr1 Ru1 32.93(13) 34 27 ?
O5 Pr1 Ru1 107.62(13) 34 27 ?
O6 Pr1 Ru1 95.56(14) 34 27 ?
O1 Pr1 Ru1 101.38(13) 2 27 ?
O1 Pr1 Ru1 33.07(13) . 27 ?
O4 Pr1 Ru1 100.35(12) 26_455 27 ?
Na1 Pr1 Ru1 56.157(13) . 27 ?
Na2 Pr1 Ru1 62.83(6) 34 27 ?
O2 Pr1 Pr2 115.33(14) 26_455 27 ?
O3 Pr1 Pr2 43.71(14) . 27 ?
O4 Pr1 Pr2 81.44(14) 34 27 ?
O5 Pr1 Pr2 115.61(14) 34 27 ?
O6 Pr1 Pr2 51.36(14) 34 27 ?
O1 Pr1 Pr2 115.79(13) 2 27 ?
O1 Pr1 Pr2 48.68(13) . 27 ?
O4 Pr1 Pr2 161.40(12) 26_455 27 ?
Na1 Pr1 Pr2 92.921(12) . 27 ?
Na2 Pr1 Pr2 62.02(6) 34 27 ?
Ru1 Pr1 Pr2 61.065(11) 27 27 ?
O2 Pr2 O3 69.36(19) 2 . ?
O2 Pr2 O5 77.9(2) 2 17_554 ?
O3 Pr2 O5 114.05(19) . 17_554 ?
O2 Pr2 O3 111.4(2) 2 26_455 ?
O3 Pr2 O3 120.92(8) . 26_455 ?
O5 Pr2 O3 123.99(18) 17_554 26_455 ?
O2 Pr2 O6 124.59(19) 2 17_554 ?
O3 Pr2 O6 84.7(2) . 17_554 ?
O5 Pr2 O6 69.27(19) 17_554 17_554 ?
O3 Pr2 O6 123.90(19) 26_455 17_554 ?
O2 Pr2 O6 130.23(19) 2 34 ?
O3 Pr2 O6 63.36(18) . 34 ?
O5 Pr2 O6 135.41(18) 17_554 34 ?
O3 Pr2 O6 81.71(19) 26_455 34 ?
O6 Pr2 O6 66.2(2) 17_554 34 ?
O2 Pr2 O1 77.26(18) 2 26_455 ?
O3 Pr2 O1 146.11(18) . 26_455 ?
O5 Pr2 O1 62.56(17) 17_554 26_455 ?
O3 Pr2 O1 66.19(18) 26_455 26_455 ?
O6 Pr2 O1 120.35(19) 17_554 26_455 ?
O6 Pr2 O1 144.91(18) 34 26_455 ?
O2 Pr2 O6 165.34(19) 2 18_554 ?
O3 Pr2 O6 124.95(18) . 18_554 ?
O5 Pr2 O6 96.76(19) 17_554 18_554 ?
O3 Pr2 O6 60.16(18) 26_455 18_554 ?
O6 Pr2 O6 64.4(3) 17_554 18_554 ?
O6 Pr2 O6 62.7(2) 34 18_554 ?
O1 Pr2 O6 88.16(17) 26_455 18_554 ?
O2 Pr2 Ru2 156.28(14) 2 16_554 ?
O3 Pr2 Ru2 90.09(14) . 16_554 ?
O5 Pr2 Ru2 101.15(14) 17_554 16_554 ?
O3 Pr2 Ru2 89.03(13) 26_455 16_554 ?
O6 Pr2 Ru2 38.10(13) 17_554 16_554 ?
O6 Pr2 Ru2 38.07(13) 34 16_554 ?
O1 Pr2 Ru2 123.78(12) 26_455 16_554 ?
O6 Pr2 Ru2 37.82(12) 18_554 16_554 ?
O2 Pr2 Ru3 37.98(14) 2 . ?
O3 Pr2 Ru3 35.62(13) . . ?
O5 Pr2 Ru3 86.55(14) 17_554 . ?
O3 Pr2 Ru3 135.46(13) 26_455 . ?
O6 Pr2 Ru3 95.49(13) 17_554 . ?
O6 Pr2 Ru3 98.76(13) 34 . ?
O1 Pr2 Ru3 113.82(12) 26_455 . ?
O6 Pr2 Ru3 156.34(12) 18_554 . ?
Ru2 Pr2 Ru3 118.537(15) 16_554 . ?
O2 Pr2 Pr1 121.35(14) 2 26_455 ?
O3 Pr2 Pr1 161.70(13) . 26_455 ?
O5 Pr2 Pr1 83.70(13) 17_554 26_455 ?
O3 Pr2 Pr1 43.11(13) 26_455 26_455 ?
O6 Pr2 Pr1 98.38(14) 17_554 26_455 ?
O6 Pr2 Pr1 101.26(13) 34 26_455 ?
O1 Pr2 Pr1 45.25(12) 26_455 26_455 ?
O6 Pr2 Pr1 44.06(12) 18_554 26_455 ?
Ru2 Pr2 Pr1 81.702(11) 16_554 26_455 ?
Ru3 Pr2 Pr1 158.985(19) . 26_455 ?
O2 Pr2 Ru1 79.59(14) 2 . ?
O3 Pr2 Ru1 138.90(13) . . ?
O5 Pr2 Ru1 30.32(13) 17_554 . ?
O3 Pr2 Ru1 94.82(13) 26_455 . ?
O6 Pr2 Ru1 91.77(14) 17_554 . ?
O6 Pr2 Ru1 149.25(13) 34 . ?
O1 Pr2 Ru1 32.72(12) 26_455 . ?
O6 Pr2 Ru1 88.96(12) 18_554 . ?
Ru2 Pr2 Ru1 111.721(13) 16_554 . ?
Ru3 Pr2 Ru1 104.71(2) . . ?
Pr1 Pr2 Ru1 59.283(12) 26_455 . ?
O4 Pr3 O4 88.40(19) 3 2 ?
O4 Pr3 O4 88.40(19) 3 . ?
O4 Pr3 O4 88.40(19) 2 . ?
O4 Pr3 O2 138.95(19) 3 . ?
O4 Pr3 O2 131.54(18) 2 . ?
O4 Pr3 O2 84.37(19) . . ?
O4 Pr3 O2 131.54(19) 3 2 ?
O4 Pr3 O2 84.37(19) 2 2 ?
O4 Pr3 O2 138.95(19) . 2 ?
O2 Pr3 O2 71.1(2) . 2 ?
O4 Pr3 O2 84.37(19) 3 3 ?
O4 Pr3 O2 138.95(19) 2 3 ?
O4 Pr3 O2 131.54(18) . 3 ?
O2 Pr3 O2 71.1(2) . 3 ?
O2 Pr3 O2 71.1(2) 2 3 ?
O4 Pr3 O5 144.69(18) 3 17_554 ?
O4 Pr3 O5 65.51(17) 2 17_554 ?
O4 Pr3 O5 68.50(18) . 17_554 ?
O2 Pr3 O5 67.29(18) . 17_554 ?
O2 Pr3 O5 71.77(18) 2 17_554 ?
O2 Pr3 O5 130.94(18) 3 17_554 ?
O4 Pr3 O5 65.50(17) 3 16_444 ?
O4 Pr3 O5 68.50(18) 2 16_444 ?
O4 Pr3 O5 144.69(18) . 16_444 ?
O2 Pr3 O5 130.94(18) . 16_444 ?
O2 Pr3 O5 67.29(18) 2 16_444 ?
O2 Pr3 O5 71.76(18) 3 16_444 ?
O5 Pr3 O5 119.963(8) 17_554 16_444 ?
O4 Pr3 O5 68.50(18) 3 18_544 ?
O4 Pr3 O5 144.69(18) 2 18_544 ?
O4 Pr3 O5 65.51(17) . 18_544 ?
O2 Pr3 O5 71.77(18) . 18_544 ?
O2 Pr3 O5 130.94(18) 2 18_544 ?
O2 Pr3 O5 67.29(18) 3 18_544 ?
O5 Pr3 O5 119.961(9) 17_554 18_544 ?
O5 Pr3 O5 119.961(8) 16_444 18_544 ?
O4 Pr3 Ru3 126.39(13) 3 . ?
O4 Pr3 Ru3 126.39(13) 2 . ?
O4 Pr3 Ru3 126.39(13) . . ?
O2 Pr3 Ru3 42.17(13) . . ?
O2 Pr3 Ru3 42.17(13) 2 . ?
O2 Pr3 Ru3 42.17(13) 3 . ?
O5 Pr3 Ru3 88.88(12) 17_554 . ?
O5 Pr3 Ru3 88.88(12) 16_444 . ?
O5 Pr3 Ru3 88.88(12) 18_544 . ?
O4 Pr3 Na2 53.61(13) 3 . ?
O4 Pr3 Na2 53.61(13) 2 . ?
O4 Pr3 Na2 53.61(13) . . ?
O2 Pr3 Na2 137.83(13) . . ?
O2 Pr3 Na2 137.83(13) 2 . ?
O2 Pr3 Na2 137.83(13) 3 . ?
O5 Pr3 Na2 91.12(12) 17_554 . ?
O5 Pr3 Na2 91.12(12) 16_444 . ?
O5 Pr3 Na2 91.12(12) 18_544 . ?
Ru3 Pr3 Na2 180.0 . . ?
O4 Pr3 Ru1 33.08(13) 3 2 ?
O4 Pr3 Ru1 72.84(13) 2 2 ?
O4 Pr3 Ru1 116.24(14) . 2 ?
O2 Pr3 Ru1 150.60(14) . 2 ?
O2 Pr3 Ru1 100.02(14) 2 2 ?
O2 Pr3 Ru1 79.51(13) 3 2 ?
O5 Pr3 Ru1 138.04(12) 17_554 2 ?
O5 Pr3 Ru1 32.81(12) 16_444 2 ?
O5 Pr3 Ru1 96.88(12) 18_544 2 ?
Ru3 Pr3 Ru1 112.842(11) . 2 ?
Na2 Pr3 Ru1 67.158(11) . 2 ?
O5 Ru1 O5 95.4(3) 17_554 . ?
O5 Ru1 O1 175.9(2) 17_554 30_455 ?
O5 Ru1 O1 85.4(2) . 30_455 ?
O5 Ru1 O1 85.4(2) 17_554 26_455 ?
O5 Ru1 O1 175.9(2) . 26_455 ?
O1 Ru1 O1 94.0(3) 30_455 26_455 ?
O5 Ru1 O4 96.8(2) 17_554 18_554 ?
O5 Ru1 O4 89.7(2) . 18_554 ?
O1 Ru1 O4 87.1(2) 30_455 18_554 ?
O1 Ru1 O4 86.3(2) 26_455 18_554 ?
O5 Ru1 O4 89.7(2) 17_554 2 ?
O5 Ru1 O4 96.8(2) . 2 ?
O1 Ru1 O4 86.3(2) 30_455 2 ?
O1 Ru1 O4 87.1(2) 26_455 2 ?
O4 Ru1 O4 170.3(3) 18_554 2 ?
O5 Ru1 Na1 132.28(17) 17_554 25_455 ?
O5 Ru1 Na1 132.28(17) . 25_455 ?
O1 Ru1 Na1 47.02(17) 30_455 25_455 ?
O1 Ru1 Na1 47.02(17) 26_455 25_455 ?
O4 Ru1 Na1 85.17(17) 18_554 25_455 ?
O4 Ru1 Na1 85.17(17) 2 25_455 ?
O5 Ru1 Pr3 47.78(17) 17_554 . ?
O5 Ru1 Pr3 92.90(17) . . ?
O1 Ru1 Pr3 128.25(16) 30_455 . ?
O1 Ru1 Pr3 90.60(16) 26_455 . ?
O4 Ru1 Pr3 144.60(17) 18_554 . ?
O4 Ru1 Pr3 42.49(15) 2 . ?
Na1 Ru1 Pr3 117.504(11) 25_455 . ?
O5 Ru1 Pr3 92.90(17) 17_554 16_554 ?
O5 Ru1 Pr3 47.77(17) . 16_554 ?
O1 Ru1 Pr3 90.61(16) 30_455 16_554 ?
O1 Ru1 Pr3 128.25(16) 26_455 16_554 ?
O4 Ru1 Pr3 42.49(15) 18_554 16_554 ?
O4 Ru1 Pr3 144.60(17) 2 16_554 ?
Na1 Ru1 Pr3 117.505(11) 25_455 16_554 ?
Pr3 Ru1 Pr3 124.99(2) . 16_554 ?
O5 Ru1 Pr1 131.77(17) 17_554 30_455 ?
O5 Ru1 Pr1 91.44(17) . 30_455 ?
O1 Ru1 Pr1 44.18(16) 30_455 30_455 ?
O1 Ru1 Pr1 90.95(17) 26_455 30_455 ?
O4 Ru1 Pr1 130.96(17) 18_554 30_455 ?
O4 Ru1 Pr1 42.09(15) 2 30_455 ?
Na1 Ru1 Pr1 59.084(13) 25_455 30_455 ?
Pr3 Ru1 Pr1 84.292(10) . 30_455 ?
Pr3 Ru1 Pr1 125.030(13) 16_554 30_455 ?
O5 Ru1 Pr1 91.44(17) 17_554 26_455 ?
O5 Ru1 Pr1 131.77(17) . 26_455 ?
O1 Ru1 Pr1 90.95(17) 30_455 26_455 ?
O1 Ru1 Pr1 44.18(16) 26_455 26_455 ?
O4 Ru1 Pr1 42.10(15) 18_554 26_455 ?
O4 Ru1 Pr1 130.96(17) 2 26_455 ?
Na1 Ru1 Pr1 59.082(13) 25_455 26_455 ?
Pr3 Ru1 Pr1 125.028(13) . 26_455 ?
Pr3 Ru1 Pr1 84.295(10) 16_554 26_455 ?
Pr1 Ru1 Pr1 118.17(3) 30_455 26_455 ?
O5 Ru1 Pr1 142.79(17) 17_554 29_455 ?
O5 Ru1 Pr1 84.76(17) . 29_455 ?
O1 Ru1 Pr1 41.22(16) 30_455 29_455 ?
O1 Ru1 Pr1 92.16(16) 26_455 29_455 ?
O4 Ru1 Pr1 45.98(17) 18_554 29_455 ?
O4 Ru1 Pr1 127.35(16) 2 29_455 ?
Na1 Ru1 Pr1 58.401(13) 25_455 29_455 ?
Pr3 Ru1 Pr1 169.302(14) . 29_455 ?
Pr3 Ru1 Pr1 60.089(8) 16_554 29_455 ?
Pr1 Ru1 Pr1 85.331(18) 30_455 29_455 ?
Pr1 Ru1 Pr1 62.805(14) 26_455 29_455 ?
O6 Ru2 O6 180.0(7) . 19 ?
O6 Ru2 O6 89.5(2) . 21 ?
O6 Ru2 O6 90.5(2) 19 21 ?
O6 Ru2 O6 90.5(2) . 3 ?
O6 Ru2 O6 89.5(2) 19 3 ?
O6 Ru2 O6 180.0(4) 21 3 ?
O6 Ru2 O6 89.5(2) . 20 ?
O6 Ru2 O6 90.5(2) 19 20 ?
O6 Ru2 O6 90.5(2) 21 20 ?
O6 Ru2 O6 89.5(2) 3 20 ?
O6 Ru2 O6 90.5(2) . 2 ?
O6 Ru2 O6 89.5(2) 19 2 ?
O6 Ru2 O6 89.5(2) 21 2 ?
O6 Ru2 O6 90.5(2) 3 2 ?
O6 Ru2 O6 180.0(3) 20 2 ?
O6 Ru2 Na2 55.10(18) . . ?
O6 Ru2 Na2 124.90(18) 19 . ?
O6 Ru2 Na2 124.90(18) 21 . ?
O6 Ru2 Na2 55.10(18) 3 . ?
O6 Ru2 Na2 124.90(18) 20 . ?
O6 Ru2 Na2 55.10(18) 2 . ?
O6 Ru2 Na2 124.90(18) . 19 ?
O6 Ru2 Na2 55.10(18) 19 19 ?
O6 Ru2 Na2 55.10(18) 21 19 ?
O6 Ru2 Na2 124.90(18) 3 19 ?
O6 Ru2 Na2 55.10(18) 20 19 ?
O6 Ru2 Na2 124.90(18) 2 19 ?
Na2 Ru2 Na2 180.0 . 19 ?
O6 Ru2 Pr2 51.48(17) . 17_554 ?
O6 Ru2 Pr2 128.52(17) 19 17_554 ?
O6 Ru2 Pr2 53.93(18) 21 17_554 ?
O6 Ru2 Pr2 126.07(18) 3 17_554 ?
O6 Ru2 Pr2 121.40(17) 20 17_554 ?
O6 Ru2 Pr2 58.60(17) 2 17_554 ?
Na2 Ru2 Pr2 71.137(7) . 17_554 ?
Na2 Ru2 Pr2 108.863(7) 19 17_554 ?
O6 Ru2 Pr2 128.52(17) . 29_445 ?
O6 Ru2 Pr2 51.48(17) 19 29_445 ?
O6 Ru2 Pr2 126.07(18) 21 29_445 ?
O6 Ru2 Pr2 53.93(18) 3 29_445 ?
O6 Ru2 Pr2 58.60(17) 20 29_445 ?
O6 Ru2 Pr2 121.40(17) 2 29_445 ?
Na2 Ru2 Pr2 108.863(7) . 29_445 ?
Na2 Ru2 Pr2 71.137(7) 19 29_445 ?
Pr2 Ru2 Pr2 180.000(15) 17_554 29_445 ?
O6 Ru2 Pr2 126.07(18) . 16_444 ?
O6 Ru2 Pr2 53.93(18) 19 16_444 ?
O6 Ru2 Pr2 121.41(17) 21 16_444 ?
O6 Ru2 Pr2 58.59(17) 3 16_444 ?
O6 Ru2 Pr2 128.52(17) 20 16_444 ?
O6 Ru2 Pr2 51.48(17) 2 16_444 ?
Na2 Ru2 Pr2 71.137(7) . 16_444 ?
Na2 Ru2 Pr2 108.863(7) 19 16_444 ?
Pr2 Ru2 Pr2 110.073(7) 17_554 16_444 ?
Pr2 Ru2 Pr2 69.927(7) 29_445 16_444 ?
O6 Ru2 Pr2 53.93(18) . 28 ?
O6 Ru2 Pr2 126.07(18) 19 28 ?
O6 Ru2 Pr2 58.59(17) 21 28 ?
O6 Ru2 Pr2 121.41(17) 3 28 ?
O6 Ru2 Pr2 51.48(17) 20 28 ?
O6 Ru2 Pr2 128.52(17) 2 28 ?
Na2 Ru2 Pr2 108.863(7) . 28 ?
Na2 Ru2 Pr2 71.137(7) 19 28 ?
Pr2 Ru2 Pr2 69.927(7) 17_554 28 ?
Pr2 Ru2 Pr2 110.073(7) 29_445 28 ?
Pr2 Ru2 Pr2 180.00(2) 16_444 28 ?
O3 Ru3 O3 98.3(2) . 2 ?
O3 Ru3 O3 98.3(2) . 3 ?
O3 Ru3 O3 98.3(2) 2 3 ?
O3 Ru3 O2 174.0(2) . 3 ?
O3 Ru3 O2 85.3(2) 2 3 ?
O3 Ru3 O2 85.8(2) 3 3 ?
O3 Ru3 O2 85.3(2) . 2 ?
O3 Ru3 O2 85.8(2) 2 2 ?
O3 Ru3 O2 174.0(2) 3 2 ?
O2 Ru3 O2 90.2(2) 3 2 ?
O3 Ru3 O2 85.8(2) . . ?
O3 Ru3 O2 174.0(2) 2 . ?
O3 Ru3 O2 85.3(2) 3 . ?
O2 Ru3 O2 90.2(2) 3 . ?
O2 Ru3 O2 90.2(2) 2 . ?
O3 Ru3 Pr3 119.10(17) . . ?
O3 Ru3 Pr3 119.10(17) 2 . ?
O3 Ru3 Pr3 119.10(17) 3 . ?
O2 Ru3 Pr3 54.89(17) 3 . ?
O2 Ru3 Pr3 54.89(17) 2 . ?
O2 Ru3 Pr3 54.89(17) . . ?
O3 Ru3 Pr2 135.55(17) . 2 ?
O3 Ru3 Pr2 45.57(17) 2 2 ?
O3 Ru3 Pr2 110.20(17) 3 2 ?
O2 Ru3 Pr2 45.42(16) 3 2 ?
O2 Ru3 Pr2 69.68(16) 2 2 ?
O2 Ru3 Pr2 128.64(17) . 2 ?
Pr3 Ru3 Pr2 75.751(18) . 2 ?
O3 Ru3 Pr2 45.57(17) . . ?
O3 Ru3 Pr2 110.20(17) 2 . ?
O3 Ru3 Pr2 135.55(17) 3 . ?
O2 Ru3 Pr2 128.64(17) 3 . ?
O2 Ru3 Pr2 45.42(16) 2 . ?
O2 Ru3 Pr2 69.68(16) . . ?
Pr3 Ru3 Pr2 75.751(18) . . ?
Pr2 Ru3 Pr2 114.150(14) 2 . ?
O3 Ru3 Pr2 110.20(17) . 3 ?
O3 Ru3 Pr2 135.55(17) 2 3 ?
O3 Ru3 Pr2 45.57(17) 3 3 ?
O2 Ru3 Pr2 69.68(16) 3 3 ?
O2 Ru3 Pr2 128.64(17) 2 3 ?
O2 Ru3 Pr2 45.42(16) . 3 ?
Pr3 Ru3 Pr2 75.751(18) . 3 ?
Pr2 Ru3 Pr2 114.150(14) 2 3 ?
Pr2 Ru3 Pr2 114.150(14) . 3 ?
O1 Na1 O1 130.8(3) 4 2 ?
O1 Na1 O1 135.4(3) 4 3 ?
O1 Na1 O1 87.10(19) 2 3 ?
O1 Na1 O1 74.6(3) 4 . ?
O1 Na1 O1 87.10(19) 2 . ?
O1 Na1 O1 87.10(19) 3 . ?
O1 Na1 O1 87.10(19) 4 5 ?
O1 Na1 O1 135.4(3) 2 5 ?
O1 Na1 O1 74.6(3) 3 5 ?
O1 Na1 O1 130.8(3) . 5 ?
O1 Na1 O1 87.10(19) 4 6 ?
O1 Na1 O1 74.6(3) 2 6 ?
O1 Na1 O1 130.8(3) 3 6 ?
O1 Na1 O1 135.4(3) . 6 ?
O1 Na1 O1 87.10(19) 5 6 ?
O1 Na1 Ru1 114.59(13) 4 26_445 ?
O1 Na1 Ru1 114.59(13) 2 26_445 ?
O1 Na1 Ru1 37.32(13) 3 26_445 ?
O1 Na1 Ru1 112.29(13) . 26_445 ?
O1 Na1 Ru1 37.32(13) 5 26_445 ?
O1 Na1 Ru1 112.28(13) 6 26_445 ?
O1 Na1 Ru1 37.32(13) 4 27 ?
O1 Na1 Ru1 112.29(13) 2 27 ?
O1 Na1 Ru1 114.59(14) 3 27 ?
O1 Na1 Ru1 37.32(13) . 27 ?
O1 Na1 Ru1 112.28(13) 5 27 ?
O1 Na1 Ru1 114.58(14) 6 27 ?
Ru1 Na1 Ru1 120.0 26_445 27 ?
O1 Na1 Ru1 112.28(13) 4 25_455 ?
O1 Na1 Ru1 37.32(13) 2 25_455 ?
O1 Na1 Ru1 112.29(13) 3 25_455 ?
O1 Na1 Ru1 114.59(13) . 25_455 ?
O1 Na1 Ru1 114.59(13) 5 25_455 ?
O1 Na1 Ru1 37.32(13) 6 25_455 ?
Ru1 Na1 Ru1 120.0 26_445 25_455 ?
Ru1 Na1 Ru1 120.0 27 25_455 ?
O1 Na1 Pr1 175.89(13) 4 2 ?
O1 Na1 Pr1 48.73(13) 2 2 ?
O1 Na1 Pr1 47.62(13) 3 2 ?
O1 Na1 Pr1 109.05(13) . 2 ?
O1 Na1 Pr1 91.63(13) 5 2 ?
O1 Na1 Pr1 88.93(14) 6 2 ?
Ru1 Na1 Pr1 66.054(7) 26_445 2 ?
Ru1 Na1 Pr1 146.341(7) 27 2 ?
Ru1 Na1 Pr1 64.760(7) 25_455 2 ?
O1 Na1 Pr1 47.62(13) 4 6 ?
O1 Na1 Pr1 88.93(13) 2 6 ?
O1 Na1 Pr1 175.89(13) 3 6 ?
O1 Na1 Pr1 91.63(13) . 6 ?
O1 Na1 Pr1 109.05(13) 5 6 ?
O1 Na1 Pr1 48.73(14) 6 6 ?
Ru1 Na1 Pr1 146.336(7) 26_445 6 ?
Ru1 Na1 Pr1 66.051(7) 27 6 ?
Ru1 Na1 Pr1 64.757(7) 25_455 6 ?
Pr1 Na1 Pr1 129.517(14) 2 6 ?
O1 Na1 Pr1 48.73(13) 4 4 ?
O1 Na1 Pr1 175.89(13) 2 4 ?
O1 Na1 Pr1 91.63(13) 3 4 ?
O1 Na1 Pr1 88.93(13) . 4 ?
O1 Na1 Pr1 47.62(14) 5 4 ?
O1 Na1 Pr1 109.05(13) 6 4 ?
Ru1 Na1 Pr1 66.052(7) 26_445 4 ?
Ru1 Na1 Pr1 64.758(7) 27 4 ?
Ru1 Na1 Pr1 146.336(7) 25_455 4 ?
Pr1 Na1 Pr1 132.106(14) 2 4 ?
Pr1 Na1 Pr1 92.256(10) 6 4 ?
O6 Na2 O6 70.7(3) 3 2 ?
O6 Na2 O6 70.7(3) 3 . ?
O6 Na2 O6 70.7(3) 2 . ?
O6 Na2 O4 119.86(19) 3 . ?
O6 Na2 O4 153.9(2) 2 . ?
O6 Na2 O4 89.65(18) . . ?
O6 Na2 O4 89.65(18) 3 3 ?
O6 Na2 O4 119.86(19) 2 3 ?
O6 Na2 O4 153.9(2) . 3 ?
O4 Na2 O4 85.3(2) . 3 ?
O6 Na2 O4 153.9(2) 3 2 ?
O6 Na2 O4 89.65(18) 2 2 ?
O6 Na2 O4 119.86(19) . 2 ?
O4 Na2 O4 85.3(2) . 2 ?
O4 Na2 O4 85.3(2) 3 2 ?
O6 Na2 Ru2 41.93(16) 3 . ?
O6 Na2 Ru2 41.93(16) 2 . ?
O6 Na2 Ru2 41.93(16) . . ?
O4 Na2 Ru2 128.50(16) . . ?
O4 Na2 Ru2 128.50(16) 3 . ?
O4 Na2 Ru2 128.50(16) 2 . ?
O6 Na2 Pr3 138.07(16) 3 . ?
O6 Na2 Pr3 138.07(16) 2 . ?
O6 Na2 Pr3 138.07(16) . . ?
O4 Na2 Pr3 51.50(16) . . ?
O4 Na2 Pr3 51.50(16) 3 . ?
O4 Na2 Pr3 51.50(16) 2 . ?
Ru2 Na2 Pr3 180.0 . . ?
O6 Na2 Pr1 45.47(13) 3 29_445 ?
O6 Na2 Pr1 101.94(17) 2 29_445 ?
O6 Na2 Pr1 111.82(19) . 29_445 ?
O4 Na2 Pr1 101.35(15) . 29_445 ?
O4 Na2 Pr1 44.84(12) 3 29_445 ?
O4 Na2 Pr1 127.94(18) 2 29_445 ?
Ru2 Na2 Pr1 86.85(10) . 29_445 ?
Pr3 Na2 Pr1 93.15(10) . 29_445 ?
O6 Na2 Pr1 101.94(17) 3 28 ?
O6 Na2 Pr1 111.82(19) 2 28 ?
O6 Na2 Pr1 45.47(13) . 28 ?
O4 Na2 Pr1 44.84(12) . 28 ?
O4 Na2 Pr1 127.94(18) 3 28 ?
O4 Na2 Pr1 101.35(15) 2 28 ?
Ru2 Na2 Pr1 86.85(10) . 28 ?
Pr3 Na2 Pr1 93.15(10) . 28 ?
Pr1 Na2 Pr1 119.702(19) 29_445 28 ?
O6 Na2 Pr1 111.82(19) 3 30_455 ?
O6 Na2 Pr1 45.47(13) 2 30_455 ?
O6 Na2 Pr1 101.94(17) . 30_455 ?
O4 Na2 Pr1 127.94(18) . 30_455 ?
O4 Na2 Pr1 101.35(15) 3 30_455 ?
O4 Na2 Pr1 44.84(12) 2 30_455 ?
Ru2 Na2 Pr1 86.85(10) . 30_455 ?
Pr3 Na2 Pr1 93.15(10) . 30_455 ?
Pr1 Na2 Pr1 119.701(19) 29_445 30_455 ?
Pr1 Na2 Pr1 119.700(19) 28 30_455 ?
O6 Na2 Pr2 99.7(2) 3 17_554 ?
O6 Na2 Pr2 50.18(15) 2 17_554 ?
O6 Na2 Pr2 44.40(15) . 17_554 ?
O4 Na2 Pr2 103.69(13) . 17_554 ?
O4 Na2 Pr2 161.10(14) 3 17_554 ?
O4 Na2 Pr2 78.99(12) 2 17_554 ?
Ru2 Na2 Pr2 57.92(8) . 17_554 ?
Pr3 Na2 Pr2 122.08(8) . 17_554 ?
Pr1 Na2 Pr2 144.58(18) 29_445 17_554 ?
Pr1 Na2 Pr2 66.31(4) 28 17_554 ?
Pr1 Na2 Pr2 59.96(4) 30_455 17_554 ?
Ru1 O1 Na1 95.7(2) 27 . ?
Ru1 O1 Pr1 107.1(2) 27 3 ?
Na1 O1 Pr1 87.08(18) . 3 ?
Ru1 O1 Pr1 102.8(2) 27 . ?
Na1 O1 Pr1 86.04(18) . . ?
Pr1 O1 Pr1 149.9(2) 3 . ?
Ru1 O1 Pr2 100.4(2) 27 27 ?
Na1 O1 Pr2 163.3(2) . 27 ?
Pr1 O1 Pr2 92.45(18) 3 27 ?
Pr1 O1 Pr2 86.07(17) . 27 ?
Ru3 O2 Pr1 160.0(3) . 27 ?
Ru3 O2 Pr2 96.6(2) . 3 ?
Pr1 O2 Pr2 103.2(2) 27 3 ?
Ru3 O2 Pr3 82.9(2) . . ?
Pr1 O2 Pr3 94.1(2) 27 . ?
Pr2 O2 Pr3 106.3(2) 3 . ?
Ru3 O3 Pr2 98.8(2) . . ?
Ru3 O3 Pr1 138.9(3) . . ?
Pr2 O3 Pr1 106.1(2) . . ?
Ru3 O3 Pr2 114.3(3) . 27 ?
Pr2 O3 Pr2 100.0(2) . 27 ?
Pr1 O3 Pr2 93.17(19) . 27 ?
Ru1 O4 Pr1 105.0(2) 3 28 ?
Ru1 O4 Pr3 104.4(2) 3 . ?
Pr1 O4 Pr3 149.4(2) 28 . ?
Ru1 O4 Na2 107.3(2) 3 . ?
Pr1 O4 Na2 88.4(2) 28 . ?
Pr3 O4 Na2 74.88(19) . . ?
Ru1 O4 Pr1 101.2(2) 3 27 ?
Pr1 O4 Pr1 93.74(19) 28 27 ?
Pr3 O4 Pr1 88.77(17) . 27 ?
Na2 O4 Pr1 149.9(2) . 27 ?
Ru1 O5 Pr2 110.4(2) . 17_554 ?
Ru1 O5 Pr1 141.3(3) . 28 ?
Pr2 O5 Pr1 105.1(2) 17_554 28 ?
Ru1 O5 Pr3 99.4(2) . 16_554 ?
Pr2 O5 Pr3 100.4(2) 17_554 16_554 ?
Pr1 O5 Pr3 88.51(17) 28 16_554 ?
Ru2 O6 Na2 83.0(2) . . ?
Ru2 O6 Pr1 166.3(3) . 28 ?
Na2 O6 Pr1 89.6(2) . 28 ?
Ru2 O6 Pr2 90.4(2) . 17_554 ?
Na2 O6 Pr2 93.0(2) . 17_554 ?
Pr1 O6 Pr2 101.5(2) 28 17_554 ?
Ru2 O6 Pr2 88.0(2) . 28 ?
Na2 O6 Pr2 169.7(3) . 28 ?
Pr1 O6 Pr2 98.2(2) 28 28 ?
Pr2 O6 Pr2 92.14(19) 17_554 28 ?
Ru2 O6 Pr2 83.59(19) . 18_544 ?
Na2 O6 Pr2 87.19(18) . 18_544 ?
Pr1 O6 Pr2 84.58(17) 28 18_544 ?
Pr2 O6 Pr2 173.9(3) 17_554 18_544 ?
Pr2 O6 Pr2 86.78(18) 28 18_544 ?
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
Pr1 O2 2.368(6) 26_455 ?
Pr1 O3 2.425(6) . ?
Pr1 O4 2.449(5) 34 ?
Pr1 O5 2.457(6) 34 ?
Pr1 O6 2.475(6) 34 ?
Pr1 O1 2.476(6) 2 ?
Pr1 O1 2.522(6) . ?
Pr1 O4 2.633(6) 26_455 ?
Pr1 Na1 3.3479(4) . ?
Pr1 Na2 3.4719(5) 34 ?
Pr1 Ru1 3.5298(6) 27 ?
Pr1 Pr2 3.5432(6) 27 ?
Pr2 O2 2.373(6) 2 ?
Pr2 O3 2.392(6) . ?
Pr2 O5 2.426(6) 17_554 ?
Pr2 O3 2.452(6) 26_455 ?
Pr2 O6 2.533(6) 17_554 ?
Pr2 O6 2.618(6) 34 ?
Pr2 O1 2.667(6) 26_455 ?
Pr2 O6 2.780(6) 18_554 ?
Pr2 Ru2 3.2367(4) 16_554 ?
Pr2 Ru3 3.3094(5) . ?
Pr2 Pr1 3.5433(6) 26_455 ?
Pr2 Ru1 3.5933(4) . ?
Pr3 O4 2.459(5) 3 ?
Pr3 O4 2.459(5) 2 ?
Pr3 O4 2.459(5) . ?
Pr3 O2 2.498(6) . ?
Pr3 O2 2.498(6) 2 ?
Pr3 O2 2.498(6) 3 ?
Pr3 O5 2.646(6) 17_554 ?
Pr3 O5 2.646(6) 16_444 ?
Pr3 O5 2.646(6) 18_544 ?
Pr3 Ru3 3.0306(12) . ?
Pr3 Na2 3.033(6) . ?
Pr3 Ru1 3.5248(5) 2 ?
Ru1 O5 1.936(5) 17_554 ?
Ru1 O5 1.936(5) . ?
Ru1 O1 1.975(6) 30_455 ?
Ru1 O1 1.975(6) 26_455 ?
Ru1 O4 1.986(6) 18_554 ?
Ru1 O4 1.986(6) 2 ?
Ru1 Na1 3.2412(8) 25_455 ?
Ru1 Pr3 3.5249(5) 16_554 ?
Ru1 Pr1 3.5297(6) 30_455 ?
Ru1 Pr1 3.5298(6) 26_455 ?
Ru1 Pr1 3.5923(6) 29_455 ?
Ru2 O6 1.997(6) . ?
Ru2 O6 1.997(6) 19 ?
Ru2 O6 1.997(6) 21 ?
Ru2 O6 1.997(6) 3 ?
Ru2 O6 1.997(6) 20 ?
Ru2 O6 1.997(6) 2 ?
Ru2 Na2 2.967(6) . ?
Ru2 Na2 2.967(6) 19 ?
Ru2 Pr2 3.2367(4) 17_554 ?
Ru2 Pr2 3.2367(4) 29_445 ?
Ru2 Pr2 3.2367(4) 16_444 ?
Ru2 Pr2 3.2367(4) 28 ?
Ru3 O3 1.950(6) . ?
Ru3 O3 1.950(6) 2 ?
Ru3 O3 1.950(5) 3 ?
Ru3 O2 2.050(6) 3 ?
Ru3 O2 2.050(6) 2 ?
Ru3 O2 2.050(6) . ?
Ru3 Pr2 3.3094(5) 2 ?
Ru3 Pr2 3.3094(5) 3 ?
Na1 O1 2.383(6) 4 ?
Na1 O1 2.383(6) 2 ?
Na1 O1 2.383(6) 3 ?
Na1 O1 2.383(6) . ?
Na1 O1 2.383(6) 5 ?
Na1 O1 2.383(6) 6 ?
Na1 Ru1 3.2411(8) 26_445 ?
Na1 Ru1 3.2412(8) 27 ?
Na1 Ru1 3.2412(8) 25_455 ?
Na1 Pr1 3.3479(4) 2 ?
Na1 Pr1 3.3479(4) 6 ?
Na1 Pr1 3.3479(4) 4 ?
Na2 O6 2.451(8) 3 ?
Na2 O6 2.451(8) 2 ?
Na2 O6 2.451(8) . ?
Na2 O4 2.529(7) . ?
Na2 O4 2.529(7) 3 ?
Na2 O4 2.529(7) 2 ?
Na2 Pr1 3.4718(5) 29_445 ?
Na2 Pr1 3.4719(5) 28 ?
Na2 Pr1 3.4719(5) 30_455 ?
Na2 Pr2 3.615(3) 17_554 ?
O1 Ru1 1.975(6) 27 ?
O1 Pr1 2.476(6) 3 ?
O1 Pr2 2.667(6) 27 ?
O2 Pr1 2.368(6) 27 ?
O2 Pr2 2.373(6) 3 ?
O3 Pr2 2.452(6) 27 ?
O4 Ru1 1.986(6) 3 ?
O4 Pr1 2.449(5) 28 ?
O4 Pr1 2.633(6) 27 ?
O5 Pr2 2.426(6) 17_554 ?
O5 Pr1 2.457(5) 28 ?
O5 Pr3 2.646(6) 16_554 ?
O6 Pr1 2.475(6) 28 ?
O6 Pr2 2.533(6) 17_554 ?
O6 Pr2 2.618(6) 28 ?
O6 Pr2 2.780(6) 18_544 ?
